Physical Origins of Thermal Properties of Cement PasteMohammad Javad Abdolhosseini Qomi,* Franz-Josef Ulm,†and Roland J.-M. Pellenq‡
Concrete Sustainability Hub, Department of Civil and Environmental Engineering,
Massachusetts Institute of Technology, 77 Massachusetts Avenue, Cambridge, Massachusetts 02139, USA (Received 18 October 2014; revised manuscript received 13 March 2015; published 17 June 2015)
Despite the ever-increasing interest in multiscale porous materials, the chemophysical origin of their thermal properties at the nanoscale and its connection to the macroscale properties still remain rather obscure. In this paper, we link the atomic- and macroscopic-level thermal properties by combining tools of statistical physics and mean-field homogenization theory. We begin with analyzing the vibrational density of states of several calcium-silicate materials in the cement paste. Unlike crystalline phases, we indicate that calcium silicate hydrates (CSH) exhibit extra vibrational states at low frequencies (<2THz) compared to the vibrational states predicted by the Debye model. This anomaly is commonly referred to as the boson peak in glass physics. In addition, the specific-heat capacity of CSH in both dry and saturated states scales linearly with the calcium-to-silicon ratio. We show that the nanoscale-confining environment of CSH decreases the apparent heat capacity of water by a factor of 4. Furthermore, full thermal conductivity tensors for all phases are calculated via the Green-Kubo formalism. We estimate the mean free path of phonons in calcium silicates to be on the order of interatomic bonds. This satisfies the scale separability condition and justifies the use of mean-field homogenization theories for upscaling purposes. Upscaling schemes yield a good estimate of the macroscopic specific-heat capacity and thermal conductivity of cement paste during the hydration process, independent of fitting parameters.
With an average annual consumption rate of 1m3 per capita, concrete is the most-used man-made material on Earth. While well known for its appreciable load-bearing capacity, concrete’s thermophysical properties are recog-nized to be important for both construction and use phases. During cement’s exothermic hydration process, thermal stresses may cause early-age cracking, which may com-promise the long-term serviceability of structures. The dimensional arguments indicate that these thermal stresses are inversely proportional to the thermal diffusivity of cement paste. During the use phase, the thermophysical characteristics of concrete (and all other construction
materials) affect the heating and cooling energy consump-tion of buildings via either heat conducconsump-tion through the envelope or the thermal mass of the buildings, i.e., the tendency of a building to maintain a constant temperature despite outdoor temperature oscillations . Both aggre-gates and the cement paste affect the thermal properties of concrete, however, the former is the dominant factor. Despite the importance of thermal properties of concrete, such studies are truly scarce and are limited to the macro-scopic measurement of thermal properties of concrete[3–6] and cement paste[7–12]. More specifically, the interplay between chemistry and molecular properties of cement paste’s constituents and their relation to macroscopic properties remain rather obscure.
This is in part associated with the hierarchical multiscale structure of cement paste. Here, by cement paste, we invoke a stoichiometric structural model of hardened cement paste rather than nonstochiometric materials found in hydrated cement systems. One can recognize at least four separate length scales in cement paste, when conceptualized in a four-level hierarchical thought model (see Fig.1). At the nanoscale, molecular properties of individual phases become available via tools of statistical physics. In this investigation, we apply these methods to both crystalline and amorphous phases, namely, alite (Ca3SiO5 or C3S), belite (Ca2SiO5or C2S), portlandite [CaðOHÞ2or CH] and calcium silicate hydrates [ðCaOÞxðSiO2Þ1ðH2OÞyor CSH], where S, C, and H, respectively, stand for SiO2, CaO, and H2O in cement chemistry notation [see Figs.1(a)and1(c)].
*Also at Department of Civil and Environmental Engineering,
Henry Samueli School of Engineering, E4130 Engineering Gateway, University of California, Irvine, Irvine, CA 92697-2175 USA.
†Also at the MultiScale Material Science for Energy and Environment, a joint MIT-CNRS laboratory at Massachusetts Institute of Technology, 77 Massachusetts Avenue, Cambridge, MA 02139, USA.
Also at the MultiScale Material Science for Energy and Environment, a joint MIT-CNRS laboratory at Massachusetts Institute of Technology, 77 Massachusetts Avenue, Cambridge, MA 02139, USA, and Centre Interdisciplinaire des Nanosciences de Marseille, CNRS and Aix-Marseille Universite, Campus de Luminy, Marseille, 13288 Cedex 09, France.
The CSH gel at the mesoscale is considered to be comprised of polydisperse nanoscale CSH particles , based on the results of neutron scattering [14,15] and statistical nanoindentation experiments[see Fig.1(b)]. The physical properties of CSH gel at the mesoscale depend on the saturation level of the interparticle spacing and can be estimated via mean-field homogenization theories . At the microscale, the CSH gel is regarded as an isotropic and homogeneous material with gel porosity that holds anhydrous cement clinkers and other hydration products together. This is consistent with a composite view of cement paste [see Fig. 1(c)]. In this sense, we regard laboratory measurements as the homogenized response of this multiscale porous composite [see Fig.1(d)].
We have previously studied mechanical properties [18–23] and diffusion dynamics  of cement paste at the molecular level. In this paper, we focus on under-standing the physical origins of macroscopic thermal properties of cement paste, starting from the atomic scale. The paper is organized in seven sections. Section II describes the molecular structures of calcium-silicate phases in cement paste and provides details of atomistic simulations. We dedicate Sec.IIIto a thorough analysis of vibrational densities of states (VDOS) of all phases, because they are at the origins of equilibrium and non-equilibrium thermal properties of materials. Subsequently, we employ VDOSs in conjunction with MD calculation in Sec. IV to measure specific-heat capacity values at constant volume and pressure. Section V highlights the nonequilibrium thermal properties of all phases at the nanoscale from equilibrium molecular dynamics using the Green-Kubo approach. In Sec.V, we also provide a full measurement of the thermal conductivity tensor, which is accompanied by a discussion of the mean free paths of phonons and their effect on the heat transport in complex
crystalline and amorphous materials. Subsequently, we use mean-field homogenization techniques in Sec. VIto provide a seamless link between the nano- and macro-scopic thermal properties, and we compare our predictions with experiments. SectionVIIdraws final conclusions and summarizes our findings.
II. METHODS A. Molecular models
The molecular structure of solid phases in hardened cement paste vary from crystalline to amorphous, depend-ing on the phase and its chemical composition. The anhydrated clinker phases (alite and belite) and portlandite are crystalline. From a crystallography viewpoint, alite is a chemically modified form of pure tricalcium silicate (C3S), exhibiting a series of reversible phase transitions upon heating and cooling . The atomic structure of alite polymorphs is similar, differing in the orientation of isolated silica tetrahedra (SiO44−), coordination of calcium (Ca2þ) and oxygen (O2−) atoms in ionic sites, and hence symmetry groups . In the present work, we choose the M3 polymorph of C3S, the most abundant polymorph in cement clinkers, refined from single crystal by de la Torreet al.. Belite is similar to alite in many aspects. It is a chemically modified form of delicacies silicate (C2S), which also exhibits a sequence of reversible phase tran-sitions with temperature. The atomic structure of belite is consisted of isolated SiO44−groups surrounded merely by Ca2þ cations. Belite has several polymorphs such as α0H, α0
L, andβ, which are derived from theαform by decreasing symmetry because of disorder in silica groups and sub-sequent modifications in calcium atoms. In the present study, we employ theβ-C2S polymorph after Midgley, as it is the most dominant polymorph in ordinary Portland FIG. 1. A four-level thought model utilized for upscaling thermal properties of cement paste from the nanoscale to engineering scale. (a) Snapshot of a nanotexture of CSH at Ca∶Si¼1.5. The brown and cyan spheres represent intra- and interlayer calcium ions. The Si—O bonds are shown by yellow-red bars. The water molecules and hydroxyl groups are depicted by red-white bars. The xy plane is parallel and the z axis is perpendicular to the calcium-silicate sheets. (b) The mesotexture of CSH constructed by agglomeration of randomly oriented CSH nanoparticles with size polydispersity. (c) The microtexture of hardened paste including anhydrous clinker phases (β-C2S and C3S), hydration products (CSH and CH), and pore space (saturated or dry). (d) The macrotexture of cement paste at the engineering scale.
cement (OPC) systems. The M3 C3S andβ-C2S phases are rarely found in pure forms and usually contain minor Al3þ, Mg2þ, and Fe3þ substitutions that modulate their stability, solubility, and chemical reactivity . These substitutions are neglected in the present study because they are attributed to a relatively small mass fraction of the OPC clinker. Beside clinker phases, portlandite (CH), one of the major hydration products in OPC systems, is also crystalline and is a fairly well-known mineral. It consists of planar Ca—O bonds with dangling hydroxyl groups pointing to the interlayer spacing. In this work, we adopt a crystalline structure of portlandite after Henderson et al.
, which identifies the position of protons via1H NMR. The nanotexture of CSH strongly depends on its chemi-cal composition. In addition to 11-Å tobermorite, we utilize a set of 150 molecular models constructed to cover a wide range of calcium-to-silicon ratios (Ca∶Si), spanning from 1.1 to 2.1[18,24]. Following a combinatorial scheme, these models are constructed by structural and chemical modi-fication of 11-Å tobermorite [33,34]. The Ca∶Si ratio of 11-Å tobermorite is systematically increased by randomly removing charge-neutralized SiO2 groups from its infi-nitely long silica chains. We create five models for each Ca∶Si ratio to ensure proper statistical sampling by altering the arrangement of vacancies. As shown in Fig.1(a), CSH consists of negatively charged defective calcium-silicate layers separated by an interlayer spacing, which is filled with water molecules and charge-balancing calcium cations. Vacancies in the silicate chains provide possible adsorption sites for water molecules. The adsorption of water molecules in defect sites is performed via grand canonical Monte Carlo (GCMC) simulation ensuring equi-librium with bulk water at constant volume and room temperature. Some of the above-mentioned adsorbed water molecules are chemically unstable and dissociate into hydroxyl groups and protons upon first-principle or reac-tive force-field modeling.REAXFFpotential is subsequently utilized to enforce reaction between the interlayer water molecules and defective calcium-silicate layers [18,35]. These molecular structures are extensively validated against nuclear magnetic resonance, elastic and inelastic neutron scattering, x-ray diffraction, and drying experi-ments (for further details on model constructions and valid-ations, see Abdolhosseini et al. [18,24]). These realistic molecular structures are consistent with the averaged stoichiometry of CaxSiO2.75ðOHÞ0Ca.85ðx−1ÞðOHÞ
1.15ðx−1Þþ0.5 ×½0.8ðx−1Þ þ0.3H2O, where x is the Ca∶Si ratio and
ðOHÞCaandðOHÞSirepresent hydroxyl groups coordinated to interlayer calcium atoms and silica groups, respectively. The collective topological observation of these 150 models indicates that, while at low Ca∶Si ratios (Ca∶Si<1.2) CSH exhibits a lamellar crystalline structure with strong transversely isotropic mechanical response; the structure of CSH at high Ca∶Si ratios (Ca∶Si>1.7) is fairly amor-phous, exhibiting isotropic mechanical properties.
B. Atomistic simulation and force fields
In this work, we use molecular dynamics (MD), energy minimization, and phonon analysis techniques to study thermal properties of clinker phases and hydration products usingLAMMPS,GULP[37,38], and a series of inhouse codes. In MD, the equations of motion are integrated via the velocity-Verlet algorithm with periodic boundary con-ditions applied in all directions. After performing extensive convergence studies, the suitable time steps are found to be as small as 0.1 fs for CSH and portlandite and 1 fs for clinker phases. For crystalline phases, we create a relatively large supercell containing roughly 1000 atoms. The sizes of CSH simulation boxes are 5 to 6 times larger than the characteristic medium-range length scale of calcium-oxide layers and silica chains. Therefore, we expect no size effect in our simulations. Initially, all CSH models and the crystalline phases are relaxed in isobaric isothermal ensem-ble (NPT) at room temperature and pressure of 0 atm. To exclude the impact of fictitious forces on the trajectories of atoms from affecting velocities and heat fluxes along the MD trajectory, further simulations are carried out in the microcanonical ensemble (NVE). In order to properly calculate the statistical errors for each model, 10 indepen-dent simulations are performed, each106 time steps long. Core-only CSH force-field (FF)  potential is used in simulations (see the Supplemental Material, Sec. A and Tables I–IV, for force-field details). To avoid the computa-tional expenses incurred by the calculation of Coulombic interactions in real and reciprocal spaces, such interactions are calculated via the Wolf method. We further inves-tigate the transferability of CSH FF potential to crystalline phases by comparing its predictions of lattice structure and mechanical properties including bulk k, shear g moduli, and with Poisson’s ratio ν, against existing experimental data[42–46](see the Supplemental Material, Sec. B and Tables V and VI, for potential validations).
III. VIBRATIONAL DENSITIES OF STATES
In dielectric solids, the atomic vibrations are at the origin of nanoscale thermal properties. At low temperatures, such vibrations are considered to be harmonic, which become progressively anharmonic with increasing temperature. These collective harmonic vibrations, the so-called phonons, are closely related to thermodynamic properties such as free energy, heat capacity, and thermal conductivity. The vibra-tional density of state, also known as the phonon density of state, over frequency gðωÞ characterizes the number of phonons having a frequency in the range ofωandωþdω,
gðωÞ ¼ 1
δðω−ωsÞ; ð1Þ where N is the number of atoms and ωs is the sth eigen vibrational frequency. The first three frequencies are neglected as they are associated with translational motion
of the solid. Within the harmonic approximation theory (i.e., small atomic displacements from equilibrium positions), gðωÞ can be computed via two different approaches. The first method is the eigenvalue decomposition of the dynami-cal matrix (EDDM), which is based on the notion of the normal mode analysis . Any atomic vibration can be considered as a linear superposition of normal modes, i.e., the eigenvectors of the dynamical matrixfen; n¼1;…; Ng,
jβ¼ω2nenpα; ð2Þ where p and q denote the atoms, α and β are the Cartesian coordinate indices, andDis the dynamical matrix defined as Dpq;αβðkÞ ¼ 1 ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ mpmq p ∂2U lat ∂α∂β eikr; ð3Þ
withmpthe mass of thepth atom,Ulatis the lattice energy, andeikris the phase factor. There are a number of possible choices for the set of k points in the first Brillouin zone, the primitive cell in the reciprocal space. The supercell of crystalline models and CSH contain, respectively, roughly 1000 and 500 atoms. Although these supercells are relatively large, a fine 15×15×15 grid of k points with the Monkhorst-Pack scheme  is utilized to ensure proper sampling of the Brillouin zone.
The second method to compute gðωÞ employs the Fourier transform of the velocity autocorrelation function (VACF) over a long-enough molecular-dynamics trajectory,
gðωÞ ¼ 1 NkBT XN j¼1 mj Z ∞ −∞hvjðtÞ·vjð0Þie iωtdt; ð4Þ whereωis the frequency,kBis the Boltzmann constant,Tis the temperature,vjðtÞis the velocity, and the dot denotes the dot product. Due to the oscillatory nature of VACF (hvjðtÞ·vjð0Þi=hvjð0Þ·vjð0Þi), femtosecond and even subfemtosecond resolution is required to fully capture gðωÞ(see VACF insets in Fig. 2).
Figures2(a),2(c),2(e), and2(g)present the VDOS of, respectively, β-C2S, C3S, CH, and a CSH model with Ca∶Si¼1.5, showing that VACF and EDDM yield almost identical results for all molecular models. To better classify the different atomic bond contribution to the VDOS in complex materials such as CSH, we divide the phonon spectrum into five distinct vibrational bands, denoted I through V in Fig.2(g). We recognize the underlying atomic and molecular vibrations populating the aforementioned bands by decomposing the VACF into its partial contribu-tions, VACFγ, where γ ¼ fSi;Ca;O;OH;H2Og. These partial contributions to VDOS are presented in Figs.2(b), 2(d), 2(f), and 2(h) for β-C2S, C3S, CH, and CSH,
60 0 20 40 80 100 120 ω (THz) Si Atoms Ca Atoms O Atoms OH Groups H2O Molecules 0.1 1 10 100 1000 t (fs) –0.250 0.250.5 0.751 VACF ω (cm-1) Si Atoms Ca Atoms O Atoms Ca Atoms OH Groups 0 5 10 15 20 25 30 35 ω (THz) Si Atoms Ca Atoms O Atoms 0.1 1 10 100 1000 t (fs) –0.250 0.250.5 0.751 VACF 1 10 100 1000 10000 t (fs) –0.250 0.250.5 0.751 VACF 1 10 100 1000 10000 t (fs) –0.250 0.250.5 0.751 VACF 0 1000 2000 3000 4000 0 400 800 1200 ω (cm-1) (g) (h) VACF Method EDDM Method I II III IV V (f) (e) (a) (b) (c) (d) EDDM Method VACF Method EDDM Method VACF Method β-C2S C3S CH CSH EDDM Method VACF Method g ( ) (arb. units) g ( ω ω ) (arb. units) g ( ) (arb. units) g ( ω ω ) (arb. units) I II III I II III I II & III V
FIG. 2. Vibrational density of state (VDOS) forβ-C2S, C3S, CH, and a CSH sample with Ca∶Si¼1.5. VDOS calculated via the eigenvalue decomposition of the dynamical matrix (EDDM) and Fourier transformation of the velocity autocorrelation function (VACF) for (a)β-C2S, (c) C3S, (e) CH, and (g) CSH. The insets shows the evolution of VACF spanning 4 orders of magnitude. Decomposition of the VDOS to contributions from different atomic and molecular species for (b)β-C2S, (d) C3S, (f) CH, and (g) CSH.
respectively. The VDOS partial contributions unanimously assert that the peak in the I band is clearly attributable to the vibration of Ca—O bonds. This is in full agreement with the near-infrared spectroscopy experiments of Yu et al.
, associating ω<400cm−1 to stretching of Ca—O bonds. Unlike Ca—O phonons, vibrations of SiO4 units extend over a large band from 0 to 35 THz. As studied in detail for amorphous silica, the Si—O frequencies in the I band are related to the acousticlike rigid-body rotation of SiO4tetrahedra units in the silica network. In the case of β-C2S and C3S, the vibrations in this band are associated with the isolated rigid-body rotation of silica monomers. In the case of CSH, however, these vibrations are related to the coupled rotation of SiO4 units in the silica chains. The simulation results indicate that the II band,
400cm−1<ω<750cm−1, is dominated by the vibration of silica tetrahedra units. This is in agreement with a midinfrared experimentrelating this band to stretching of Si—O bonds, and symmetric and asymmetric bending of Si—O—Si angles. For silica glass, Taraskin and Elliot suggested that the vibrations in this frequency window are associated with a complex hybridization of acoustic and optical modes manifested in quasilocalized internal stretch-ing and bendstretch-ing of SiO4units. Furthermore, the III band in the range of750cm−1<ω<1200cm−1is also populated with silica tetrahedra vibrations. In β-C2S and C3S, these vibrations are accumulated into peaks that are associated with highly localized longitudinal and transverse optical modes that correspond to stretching and bending of silica monomers. In particular for CSH, the III band is mainly associated with the vibration ofQ1andQ0sites containing silanol groups (Si—OH), due to the strong presence of an OH signal in the partial VDOS. The vibrational frequencies in region IV result from the inplane bending of the H—O—H angle of water molecules because this vibrational frequency is only present in the partial VDOS of water molecules and it is absent in VDOS of portlandite. The V band represents both the symmetric and asymmetric stretching of O—H bonds in water molecules, the stretch-ing of hydroxyl groups coordinated to both Ca and Si atoms in CSH, and the stretching of hydroxyl groups in portlandite.
One of the most striking features in VDOS of glasses, and glass-forming and supercooled liquids is the presence of a universal excess of states (EOS) compared to that predicted by the Debye model (gD ∝ω2) in the low-frequency region . This EOS is responsible for the anomalies of the heat capacity and thermal conductivity of glasses at low temperatures . Highlighted by a broad peak in the THz region (<5THz) when plottinggðωÞ=ω2, this peak is referred to as the boson peak (BP). The BP can be experimentally identified via Raman spectroscopy and one-phonon scattering cross section in inelastic neutron scattering. Despite decades of work, the origin of BP remains an open question in condensed matter physics and
material science. Existing theoretical models explain BP via different mechanisms such as phonon-saddle transition in the energy landscape , local vibrational modes of clusters , locally favored structures , liberation of molecular fragments [58,59], vibrations in anharmonic potentials , and anomaly in transverse phonon propagation related to the Ioffe-Regel limit. Exhibiting common features of disordered and amorphous materials [18,19], the VDOS of CSH presents a BP in the THz region as shown in Fig.3. The BP is characterized by the peak position ωBP and the peak intensity IBP. As observed in many glass-forming materials such as poly-butadiene, polystyrene, LiCl, and B2O3,ωBP is usually found to be shifted to lower frequencies with increasing temperature. As an exception to this rule, ωBP in silica is slightly shifted to the left with decreasing density[64,65]. The analysis of all CSH models indicates that the composition affects both positions and intensities of BPs. When expressed in terms of density in the inset of Fig.3, ωBP of CSH decreases with increasing density and itsIBPbehaves conversely. The correlation between the CSH density and its BP properties are analogous to the pressure dependence of the BP observed in silica , Na2FeSi3O8 , and polymers.
IV. NANOSCALE HEAT-CAPACITY CALCULATIONS
Heat capacity is a thermal property of materials at equilibrium that links variations of internal energy (U) and temperature. The internal energy of an insulating solid is the sum of lattice (Ulat), vibrational (Uvib), rotational (Urot), and translational (Utra) energetic contributions. At low temperatures, considerably below the Debye tem-perature, the rotational and translational contributions
ρ (g/cm3) 1 1.5 2 2.5 ω BP (THz) 0 200 400 600 ω (cm-1) VDOS( ω)/ ω 2 (arb. units) 2.3 2.4 2.5 2.3 2.4 2.5 ρ (g/cm3) IBP (arb. units) 0 5 10 15 20 ω (THz) ωBP I BP
FIG. 3. Boson peak identification in a CSH sample with Ca∶Si¼1.5. The inset shows the location (ωBP) and intensity
(IBP) of the boson peaks for all 150 CSH models in terms of their
(Urot and Utra) are negligible compared to the other two components; hence,U≃UlatþUvib.Uvibcan be described as the number of phonons occupying a particular statenðωÞ times their vibrational energy level hω, that is,
Uvib¼ Z ∞ 0 hω nðωÞ þ1 2 dω; ð5Þ
wherehis the Plank constant andhω=2 is the zero-point energy contribution. Following Bose-Einstein statistics, fBEðωÞ ¼ ðe−hω=kBT−1Þ−1 is the probability distribution
of a boson particle occupying a specific quantum state in the thermal equilibrium. Thus, the occupation level is the degeneracy of the vibrational state, described throughgðωÞ, times the probability of the presence of phonons at that specific state; i.e., nðωÞ ¼gðωÞfBEðωÞ. This yields the kinetic energy in terms of vibrational density of states in Eqs. (1) and (4). The specific-heat capacity at constant volume can then be calculated from cv¼ ð∂U=∂TÞv¼
ð∂Uvib=∂TÞv, noting that Ulat does not depend on T at constant volume. Experimental measurement ofcvis rather difficult because it requires maintaining constant volume throughout the experiment. Therefore, laboratory measure-ment of specific-heat capacity at constant pressure cp is more popular. From thermodynamics, cv and cp are related via
where ρis the density calculated in atomistic simulation, α¼ ð1=VÞð∂V=∂TÞP is the coefficient of thermal expan-sion, and β¼−ð1=VÞð∂V=∂PÞT is the compressibility which is the reciprocal of bulk modulus. Here, we calculate these two coefficients via a finite difference approach in an isobaric-isothermal (NPT) ensemble. To this end, three 10-ns-long simulations are performed on a number of CSH samples,β-C2S, C3S, and CH at (300 K, 0 atm), (310 K, 0 atm), and (300 K, 100 atm). The results forβ-C2S, C3S, CH, 11-Å tobermorite, and a CSH model with stoichiom-etry of C1.75SH2.0 are summarized in Table I. The com-pressibility of the crystalline phases presented in the Supplemental Material , Table II, are almost identical with those calculated at zero temperature. The densities of the crystalline phases are compared to experimental values
of bulk measurements  and crystallographic density [27,29,32]. Since the effect of porosity and impurities are neglected in our atomistic simulations, our predicted densities are closer to crystallographic measurements than bulk measurements. The CSH compressibility increases with increasing Ca∶Si ratio, 1.5×10−11 Pa−1<βCSH< 1.8×10−11 Pa−1. These results are in full agreement with zero-temperature calculations of CSH’s bulk modulus kCSH, indicating a decrease in kCSH with increasing Ca∶Si ratio, 55GPa < kCSH <65GPa. CSH’s coeffi-cient of thermal expansion calculated from MD is
4.5ð0.9Þ×10−5K−1, in agreement with 4.2×10−5 K−1 microthermoporomechanics backanalysis . The CSH density is found to decrease with increasing Ca∶Si ratio,
2.55g=cm3>ρCSH>2.35g=cm3. At a low Ca∶Si ratio, the density is close to that of experimental density reported for tobermorite minerals [71,72]. The density of CSH at a high Ca∶Si ratio is slightly lower than values obtained from neutron scattering experiments[14,73]and is close to recent experimental values reported by Mulleret al. , after subtracting the monolayer of water adsorbed on the external surface of CSH nanoparticles. Having computedα, β, andρ, the difference betweencp andcvis calculated to be in the range of0.002–0.025J=g K for different calcium-silicate systems.
Table I presents the specific-heat capacities at constant volume and pressure for β-C2S, C3S, and CH. The atomistic simulation predictions of constant-pressure heat capacities are in very good agreement with low-temperature heat-capacity measurements  and with values calcu-lated from fitted cp-T relations . We regard this agreement as further validation of the transferability of CSH FF potential to other calcium-silicate systems that allows refining not only structural but also vibrational properties. Figure4 displays the specific-heat capacity of both dry (all molecular interlayer water removed)cdryv;pand hydrated chydv;p CSH in terms of the Ca∶Si ratio. The specific-heat capacities in both dry and hydrated samples increase almost linearly with Ca∶Si with a minor scatter attributable to the polymorphic structure of CSH . Similar to the experimentally observed increase in heat capacity of rocks  and Vycor glass , the heat
TABLE I. Equilibrium properties of β-C2S (belite), C3S (alite), CH (portlandite), C1.0SH0.5 (11-Å tobermorite), and C1.75SH2.0 including density, compressibility, coefficient of thermal expansion, constant-volume, and constant-pressure specific-heat capacities calculated using CSH FF potential and compared against available experimental measurements.
cv ðJ=g KÞ ρðg=cm3Þ β ð1=PaÞ αð1=KÞ cp ðJ=g KÞ
Sim. Sim. Expt. Sim. Sim. Sim. Expt.
β-C2S 0.69 3.55 3.31, 3.36 8.18×10−12 4.99×10−5 0.72 0.71, 0.75 C3S 0.68 3.57 3.13, 3.55 9.53×10−12 4.95×10−5 0.71 0.72, 0.75 CH 1.14 2.25 2.25, 2.08 3.47×10−11 9.91×10−5 1.14 1.15 C1.0SH0.5 0.87 2.55 2.48, 2.46 1.47×10−11 4.50×10−5 0.89
capacity of hydrated CSH is higher than that of dry samples. The constant-pressure specific-heat capacities can be written in the form of cdryp ¼0.66xþ0.75 and chydp ¼1.00xþ0.75, wherexis the Ca∶Si ratio. The two lines intersect at 0.75J=g K at Ca∶Si¼0, which is the experimental heat capacity of amorphous silica (devoid of calcium) at room temperature . The specific-heat capacity of CSH is less than those observed for cement pastes with different water-to-cement ratios and saturation degree. The heat capacity of cement paste is a composite response of different phases, including anhydrous clinker, portlandite, and water, that is discussed in Sec. VI.
The difference between dry and hydrated samples indicates the effect of interlayer water on the heat capacity of CSH. In fact, the apparent heat capacity of nanoconfined water can be considered as the difference between the specific-heat capacities of wet and dry CSH, Δcp¼ chydp −cdryp ¼0.34x. According to the average chemical composition (see Sec. II A), the interlayer water content scales with ΔMw¼0.8x. Since Δcp=ΔMw<1, the heat capacity of the nanoconfined water decreases with an increasing Ca∶Si ratio. It is instructive to display the variation of the heat capacity of nanoconfined water in terms of its Voronoi density rather than the Ca∶Si ratio. To this end, the Voronoi density of interlayer water is measured via a Voronoi tessellation algorithm, which finds a portion of space that is closer to a given water molecule than any other atom in the molecular structure [24,79]. The inset of Fig.4shows the relation between the normalized apparent heat capacity and the Voronoi density of the nanoconfined water. The heat capacity of water in the ultraconfining interlayer spacing of CSH (d <1.0nm) is noticeably smaller than that of bulk water at room temper-ature, roughly4.2J=g K. This is in full agreement with
Bentz’s postulate stating that the heat capacity of chemically and physically bound water within the hydration gel should be significantly lower than that of bulk water. Similar to dynamical properties, the heat capacity of nanoconfined water in CSH and its trend with density behaves like supercooled water. In fact, although being at room temper-ature,Δcp is on the order of those observed at 150 K. This is mainly due to the strong interactions between the water molecules and the substrate.
V. NANOSCALE HEAT-CONDUCTIVITY CALCULATIONS
The thermal conductivityKof a dielectric material is a second-order tensor relating the temperature gradient∇T to the heat fluxq through Fourier’s law,q¼K·∇T. There are three methods to calculateKfor an insulating solid via MD simulation: the equilibrium Green-Kubo method (GK); direct application of Fourier’s law within a steady-state conduction regime in a nonequilibrium framework (known as the direct method); and a transient nonequilibrium method. In this work, the GK approach is employed because it is less size dependent, does not involve imposing unrealistic temperature gradients in the simulation cell, and it yields the full thermal-conductivity tensor. Heat flux in a multiparticle system can be simply written as
q¼ 1 V d dt XN i¼1 riHi; ð7Þ whereriandHistand for, respectively, the position vector and the total Hamiltonian (kinetic plus potential energies) of theith particle in the system, whereasV is the volume. To exclude the numerical errors arising from the calculation of a time derivative in the finite-difference approach, the above expression can be rearranged considering the mathematical form of the interatomic potential. Assuming that the angular contributions in the CSH FF potential are equally distributed among all atoms in a water molecule,Hi can be expressed in terms of its components via
Hi¼ 1 2mivi·viþ 1 2 X j u2ðrijÞ þ 1 6 X kj u3ðθjikÞ; ð8Þ
where vi is the velocity of ith particle, u2 represents pairwise energy terms between the ith particle and its jth neighbor locatedrijapart from each other, and includes van der Waals, Coulomb interactions via Wolf summation method, and bond-stretching terms. The u3 energy term considers the bending energy of the central θijk angle in water molecules. By substituting Eq. (8) in Eq. (7), an alternative expression for heat flux is achieved,
q¼ 1 V XN i¼1 ½eivi−VSi·vi; ð9Þ 0.8 0.9 1 cp (J/g K) 0.9 0.95 1 1.05 1.1 1.15 0.2 0.24 0.28 0.32 0 0.4 0.8 1.2 1.6 2 Ca:Si 0.7 0.8 0.9 1 cv (J/g K) Hydrated CSH Dry CSH
Exp. silica: Hemingway
H 2O Density (g/cm 3 ) C p of Confined / Bulk H 2 O 11-Å Tobermorite
FIG. 4. The effect of Ca∶Si ratio on specific-heat-capacity values at constant volume and pressure for dry and hydrated CSH models and 11-Å tobermorite. The black and blue lines are fitted to the atomistic simulation data. These lines intersect at a point corresponding to the heat capacity of amorphous silica. The inset indicates the relation between the Voronoi density of the nanoconfined water and its apparent heat capacity measured as the difference between the heat capacity of dry and hydrated CSH.
where ei is the kinetic energy andSi is the atomic virial stress tensor, which can be expressed in terms of two- and three-body potential terms as
Si¼ 1 2V X Np;Nb j¼1 rij⊗Fijþ 1 6V XNa i¼1
ðrijþrikÞ⊗Fijk; ð10Þ where ⊗is the dyadic product in tensor notation,Fij the force due to pair potentials, and Fijk¼−∇iu3ðθjikÞ is a three-body force term. We implement the above heat-flux formulation in GULP source code[37,38]. In equilibrium, the net heat flux qðtÞ fluctuates around zero along the molecular-dynamics trajectory. To measure thermal con-ductivity at equilibrium, the GK approach links K to the dissipation rate of heat-flux fluctuations at the atomic scale via the fluctuation-dissipation theorem. The GK formalism for an anisotropic material can be written as
0 hqðtÞ⊗qð0Þidt; ð11Þ
where Ψ¯ðtÞ ¼ hqðtÞ⊗qð0Þi=hqð0Þ⊗qð0Þi is a second-order tensor generally known as the heat-flux autocorre-lation function (HFACF). HFACF elements are one at the origin and subsequently decay to zero with characteristic time scales proportional to the thermal conductivity of the material. Since the length of the MD trajectory is finite, numerical estimation ofKis usually truncated aftertM, the time corresponding to convergence of HFACF to zero, and it is calculated via  KijðtMÞ ¼ ΔtV kBT2 XM m¼1 1 s−m Xs−m n¼1 qiðmþnÞqjðnÞ hqið0Þqjð0Þi ; ð12Þ
where Δt is the heat-flux outputting time step, which is different from the molecular-dynamics time stepδt;sis the total number of output steps;tMis given byMΔt; andqjðnÞ is thejth component of the heat flux at thenth output step. A number of complications arise when calculating the thermal conductivity using Eq.(12). Due to the finite value of s, imposed by limitations on the disk space and computational expense, thermal conductivity might be erroneously shown to be nonsymmetric. However, K is mathematically shown to be both positive semidefinite and symmetric [86,87]. This is an artifact of the numerical calculation of HFACF,ϵ¼ jΨij¯ ðtÞ−Ψji¯ ðtÞj>0jfori≠j. ϵ can be minimized by increasing s, which requires excessive computational expense. Another way to exclude ϵis to enforce symmetry viaΨij ¼ ðΨij¯ þΨji¯ Þ=2. In fact, the ergodicity of equilibrium processes requiresΨij¯ ¼Ψji¯ and, therefore, enforcing symmetry is meaningful. Also, as shown in the insets of Figs.5(a)–5(d), some oscillations of HFACF might still be present at large time scales
(t >105 fs). To better understand the nature of these
oscillations, we note that the GK relation [Eq. (11)] can be expressed in the frequency domain,
KðωÞ ¼ V
iωtdt; ð13Þ where the thermal conductivity can be regarded as the limit of KðωÞ at zero frequency. Figures 5(a)–5(d) present different elements of KðωÞ for β-C2S, C3S, CH, and a CSH molecular structure with Ca∶Si¼1.5. It is noted that the high frequencies in the IV and V bands defined in VDOS (Fig.2) are absent inKðωÞ. This simply means that the hydroxyl groups and water molecules do not contribute to the oscillations of heat conduction. This is due to the dangling nature of hydroxyl groups, which do not con-tribute to the propagation of phonons, as discussed later in this section. In the case ofK11andK22forβ-C2S and C3S, the contributing frequencies to the oscillation of thermal conductivity extend over the I, II, and III bands and exhibit distinct peaks. By decomposing Eq.(7) intoqu¼
ð1=VÞPNi¼1viUiandqk¼ ð1=VÞ PN
i¼1riU_i, Landryet al. associated the oscillation inKðtÞto optical zero-wave vector phonons. This explanation is consistent with our observation of the absence of such peaks at low frequencies in β-C2S and C3S pertaining to the longitudinal and transverse acoustic phonons. The heat conduction across the interlayer spacing of CH and CSH is more sophisti-cated. The absence of bonded interaction between the layers, also evidenced in elastic properties (C11> C33
and C22> C33 following Voigt notation), makes the
measurement of K33 more complicated. In Figs.5(c)and 5(d), the optical zero-wave vector phonons contributing to the oscillations of K33ðωÞ are only present at two sharp peaks in the I and II bands. Unlike β-C2S and C3S, significant peaks, however, emerge at low frequencies. This is the evidence of a complex interplay between acoustic and optical phonons which has also been observed in the study of VDOS of amorphous silica. As shown in the enlarged insets of Figs. 5(a)–5(d), KiiðωÞ decays smoothly at small enough frequencies to its limit value. To estimate this limit thermal conductivity (kij), we fitted a power function of the formKijðωÞ ¼Kijþξωζ, where Kij,ξ, andζare estimated using the least-squares approach. In addition, ten independent simulations with different initial conditions are performed for each molecular model, and the mean and standard deviation of the thermal-conductivity tensor are computed subsequently. Each simulation is 10 ns long, and qðtÞ is recorded every 0.1 fs for CH and CSH, and every 1.0 fs for β-C2S and C3S. The thermal conductivity calculated using this method is found to be close to the average value of thermal conductivity in the time domain. A particularity of CSH is that the value of thermal conductivity depends onΔt, the resolution in which qðtÞ is recorded. In fact, the HFACF plunges very quickly to zero, meaning that the assessment of short time-scale behaviors ofΨðtÞis crucial. To this end,
we measured the thermal conductivity of CSH with differ-entΔt resolutions using the above method. The true thermal conductivity of CSH is then the limit of KijðΔtÞ for vanishingΔtvalues. Specifically, we find that the thermal conductivity of CSH scales linearly with Δt, KijðΔtÞ ¼ ζΔtþK0ij, so that the intercept at the origin can be consi-dered to be the actual thermal conductivity of CSH;
Following the above procedure, the full thermal-conductivity tensor is computed for all models. In the case ofβ-C2S and C3S, we findKto be diagonal (Kij ¼0; i≠j). Therefore, the , , and  are the same as the principal thermal-conductivity directions. For the CH and CSH models, we generally find thatK11> K22> K12 andK12 ≫K013; K023. Therefore, the thermal conductivity of CH and CSH in a Cartesian coordinate system, where 1, 2, and 3 directions are, respectively, , , and  crystallographic directions, can be approximated as
K≃ 2 6 4 k11 k12 0 k12 k22 0 0 0 k33 3 7 5: ð14Þ
This form of the thermal-conductivity tensor presented in Eq. (14) is not only symmetric but also positive-definite
because of the magnitude of theKij elements. The tensor of thermal conductivity can be expressed in terms of its principal thermal conductivities, the eigenvalues of theK tensor. The principal thermal-conductivity values forβ-C2S, C3S, CH, 11-Å tobermorite, and a CSH model are summa-rized in TableII. The three principal conductivity values for CSH models, KIII< KII< KI, are presented in Figs. 5(a)–5(c). While the eigenvectors corresponding to KI and KII are located in the 12 plane (calcium-silicate layers), the third axis (across the interlayer spacing) is fully aligned with the eigenvector associated withKIII. Akin to the anisotropic nature of mechanical properties of CSH, the heat-transport properties also show strong anisotropy such that the thermal conductivity in the defective calcium-silicate sheets (12 plane) is statistically larger than that of the out-of-plane direction (third axis). While the xy plane is populated with fairly heat conductive Si—O bonds, looser Ca—O bonds and water molecules in the interlayer space scatter phonons and diminish the heat transport along the zdirection, perpendicular to the layers.
Despite the clear presence of anisotropy in heat-transport properties, we find no correlation between the chemical composition and thermal conductivity of CSH in Fig.6. To this end, we investigate the absence of such correlation via a comparative analysis with crystalline phases. The volume 0 200 400 600 800 | K11 ( ω) | (W/m K) 1 10 100 100010000 t (fs) 0 20 40 K33 (W/m K) -0.5 0 0.5 1 HFACF 11 1 10 100 1000 10000 t (fs) -20 0 20 40 K11 (W/m K) 0 1000 2000 3000 | K33 ( ω) | (W/m K) 0.1 1 10 100 1000 t (fs) -10 0 10 K33 (W/m K) -0.5 0 0.5 1 HFACF 33 ω (cm-1) 0 400 800 1200 0 400 800 1200 ω (cm-1) 0 5 10 15 20 25 30 35 ω (THz) 0 100 200 300 400 500 | K22 ( ω) | (W/m K) -0.5 0 0.5 1 HFACF 22 1 10 100 1000 10000 t (fs) -20 0 20 40 K33 (W/m K) 0 5 10 15 20 25 30 35 ω (THz) 0 50 100 150 200 | K33 ( ω) | (W/m K) HFACF 0 33 Fit β-C2S III II I CH I II III | K33 (0) | |K 11(0) | Fit C3S Fit |K22(0) | III II I (a) CSH III II I (b) (c) (d) Fit |K33(0) |
FIG. 5. The power spectra of different components of the thermal conductivity tensor in frequency domain (Fourier transform of the heat-flux autocorrelation function) forβ-C2S, C3S, CH, and a CSH sample with Ca∶Si¼1.5. The insets in black and red correspond to the heat-flux autocorrelation function and the thermal conductivity in time domain, respectively, exhibiting pronounced oscillations in long time-scales. The enlarged inset shows the fitting procedure adopted here to estimate the thermal conductivity at the zero frequency which corresponds to Green-Kubo relation.
thermal conductivity of CSH does not alter with the Ca∶Si ratio and it is close to that of 11-Å tobermorite (see Table II). The above Kv values for CSH are close to those of amorphous silica measured experimentally [89–93]and calculated numericallyand theoretically [95,96]. Since the variation of the Ca∶Si ratio is merely achieved by removing SiO2groups from 11-Å tobermorite, it can be viewed as a parameter that is inversely propor-tional to the defect content. In the absence of an interface and boundaries in the bulk material, there are two phonon scattering mechanisms: phonon-phonon and phonon-defect scattering. Assuming that different scattering processes are independent, Matthiessen’s rule combines the two scatter-ing mechanisms to an effective process usscatter-ing
1 lm ¼¯ 1 lph-vacancy þ¯ 1 lph-ph ; ð15Þ
wherelm is the mean free path of phonons and¯lph-vacancyis the mean phonon-vacancy scattering length, the distance that a phonon travels prior to being scattered off a vacancy defect.¯lph-phis the mean phonon-phonon scattering length, the distance that a phonon travels before being scattered by another phonon. Matthiessen’s rule specifies two limiting regimes for phonon transport in a material: vibration-dominated (¯lph-ph≪¯lph-vacancy) and defect-dominated
(¯lph-vacancy≪¯lph-ph) regimes. Therefore, if a material is in the vibration-dominated regime, then the population of defects would not affect the heat-transport properties. Here, the kinetic theory formulation of heat transport can be used to estimate the characteristic length scale of phonons,
whereSvis the speed of sound estimated by averaging the longitudinal and transverse sound velocities, Sl and St, respectively, using Sv¼ 1 3 1 S3l þ 2 S3t −1=3 ; ð17Þ whereSl¼ ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ð4gþ3kÞ=3ρ p andSt¼ ﬃﬃﬃﬃﬃﬃﬃﬃ g=ρ p
are the poly-crystalline averages of these acoustic velocities computed from the bulk k and shear g moduli and the density presented in TableI and the Supplemental Material , Table VI. The acoustic velocities and mean free path of phonons forβ-C2S, C3S, CH, 11-Å tobermorite, and a CSH model are provided in TableII. The mean free path of CSHs and CH is almost half of that ofβ-C2S and C3S. The space-filling structure of the clinker phases explains their rela-tively high thermal conductivity and the mean free path of TABLE II. Transport properties of β-C2S (belite), C3S (alite), CH (portlandite), C1.0SH0.5 (11-Å tobermorite), and C1.75SH2.0
including principal thermal conductivity values, volumetric thermal conductivity, longitudinal, transverse, and volumetric acoustic velocities, and the mean free path of phonons calculated using CSH FF potential.
KI ðW=m KÞ KII ðW=m KÞ KIIIðW=m KÞ Kv ðW=m KÞ Sl ðkm=sÞ St ðkm=sÞ Sv ðkm=sÞ lm (Å) β-C2S 3.450.4 3.450.4 3.450.4 3.450.4 21.4 12.0 13.3 3.2 C3S 3.350.3 3.350.3 3.350.3 3.350.3 22.4 12.6 14.0 2.9 CH 2.000.2 1.200.2 0.750.2 1.320.2 14.1 7.0 7.9 1.7 C1.0SH0.5 1.250.2 0.950.2 0.740.2 0.980.2 19.9 10.2 11.4 1.4 C1.75SH2.0 1.250.2 0.950.2 0.740.2 0.980.2 19.2 11.67 12.9 1.6 1.2 1.6 2 Ca:Si 0 0.4 0.8 1.2 1.6 2 Principal K (W/m K ) 1.2 1.6 2 Ca:Si 1.6 1 1.2 1.4 1.8 2 Ca:Si 0 1 2 3 lm (Å) C-S-H 1.2 1.6 2 Ca:Si
Amorphous Silica: Cahill et al.
KIII KII KI
Amorphous Silica :
Ratcliffe et al.
Cahill et al. Si—O bond length
Ca—O bond length
FIG. 6. The anisotropic nature of thermal conduction in CSH and the effect of stoichiometry on the principal thermal conductivity values (a)KI, (b)KII, and (c)KIIIcompared against the experimental values of thermal conductivity of amorphous silica measured by
Cahillet al.and Ratcliffe. (d) The mean free path of phonons (lm) in CSH compared against mean free path of phonons in amorphous silica as measured by Cahillet al.[89,91], Ca—O and Si—O bond lengths.
the phonons. The thermal conductivity values observed forβ-C2S and C3S are close to the thermal conductivity of crystalline silica . However, the layered structure of CSH and CH scatters phonons across the interlayer spacing and significantly reduces the heat transport properties. In fact, lm is on the order of Si—O and Ca—O bond lengths (dSi—O¼1.62Å anddCa—O¼2.42Å) across the range of considered Ca∶Si ratios in CSH, which agrees with experimental measurements of Cahillet al.[89,96]for fused silica. Therefore, it can be safely assumed that heat transport in CSH and CH is in the vibration-dominated regime [Fig.6(d)]. This explains why the Ca∶Si ratio (or, in other words, the defect content) does not significantly alter the thermal conductivity of CSH. Moreover, the absence of a phonon-defect-scattering mechanism satisfies the scale separability condition and justifies the use of mean-field homogenization theories for upscaling purposes.
VI. MACROSCALE THERMAL PROPERTIES
In Secs.IVandV, we explored the effect of chemistry on the nanoscale equilibrium and nonequilibrium thermophys-ical properties of various calcium-silicate phases present in cement paste. In this section, we employ multiscale modeling techniques to link the nanoscale properties of individual constituent phases of cement paste to macroscale properties [79,99–103]. The upscaling of specific-heat capacity from the atomic scale (level 0) to the macroscale (level 3) is rather straightforward. Since energy and volume are extensive thermodynamic quantities, they can be written as the sum of those quantities for individual phases in a composite material. Therefore, the constant-pressure specific-heat capacity of a composite can be considered as a linear combination of that of individual phases. This also holds true during the course of chemical reaction involving m reactive agents (Ri) andnreaction products (Pi),
α1R1þ þαmRm→β1P1þ þβnPn; ð18Þ where αi and βi are the number of moles of reactants and products in the balanced stoichiometry, respectively. Investigations on the properties of a mixture of reactants and products can be performed in terms of reaction degree η, i.e., the mass of reactants at a given time divided by the total mass of reactants and products. Hence, the constant-pressure specific-heat capacity of a mixture of reactants and products in terms of reaction degree can be written as
cmixp ¼ ð1−ηÞ Xm i¼1 ϕRic Ri p þη Xm i¼1 ϕPic Pi p; ð19Þ where cRi
p and cPpi are constant-pressure specific-heat capacities of, respectively, the ith reactant and product. ϕRi¼αiMRi=
mass fractions of the ith reactant and product with molar mass MRi and MPi, respectively. Traditionally, cement
paste is regarded as a composite of anhydrous clinker phases and hydration products that, in the case of CSH, is a nonstoichiometric product . To simplify the complex cement hydration reaction, we assume a constant stoichi-ometry for the resultant CSH. Therefore, the hydration process is written as
C2SþzH→C1.7SH1.9þ0.3CHþ ðz−2.2ÞH; ð20Þ C3SþzH→C1.7SH1.9þ1.3CHþ ðz−3.2ÞH; ð21Þ wherezis the number of water moles used in the hydration and C1.7SH1.9is the common form of CSH in OPC systems. In the current work, we neglect the impact on thermal properties of cement paste from aluminate phases such as C3A and C4AF and their hydration products.
By juxtaposing Eqs. (18)–(21) and using the specific-heat-capacity values provided in Table I, the constant-pressure specific-heat capacity of hydrating cement paste can be estimated in terms of hydration degree. Figure 7 presents the constant-pressure specific-heat capacities of three hydrating cement pastes with water-to-cement ratios (w=c) of 0.3, 0.4, and 0.5 and their comparison with macroscopic experimental measurements of Bentz . According to Eq. (19), simulation results are necessarily linear in terms ofηand are in qualitatively good agreement with the experimental measurements. The slight difference between the experiment and simulation are attributed to the presence of other phases in OPC systems and the difference between the properties of bulk and interfacial water. Nevertheless, both simulation and experiments indicate that the heat capacity of the paste decreases with increasing hydration degree. This can be understood by proper consideration of the role of water during the course of hydration. The specific-heat capacity of bulk water is considerably high (4.18J=g K), which makes the heat
0 0.2 0.4 0.6 0.8 1 η: Hydration Degree 1 1.2 1.4 1.6 1.8 2 2.2 cp (J/g K) Sim. w/c=0.3 Sim. w/c=0.4 Sim. w/c=0.5 Exp. w/c=0.3 Exp. w/c=0.4
FIG. 7. The effect of hydration degree on the macroscopic specific-heat capacity of hydrating cement paste for three water-to-cement ratios (w=c). The simulation results derived from atomistic simulation and mixture laws are compared with experimental measurements of Bentzforw=c¼0.3and 0.4.
capacity of the mixture of water and clinker relatively high. Throughout the hydration process, the water is consumed to precipitate CSH, which has significantly lower specific-heat capacity (see Fig.4). Also, part of this water is trapped within the CSH molecular structure, which exhibits fea-tures of supercooled water with considerably lower spe-cific-heat capacity compared to that of room-temperature bulk water (see the inset of Fig. 4). Following the same lines of thought, we infer that the heat capacity of cement paste increases with increasingw=cratio. This is confirmed by both simulation and experiment and can be rationalized in the sense that the portion of water that does not contribute to hydration is trapped in the interparticle and capillary pores. The large specific-heat capacity of unreacted water in such pores increases the heat capacity of the cement paste.
Since heat flux is an intensive thermodynamic quantity, simple composition-based mixture rules are not suitable for upscaling heat-transport properties in composite materials. Fortunately, mean-field homogenization theories present a consistent mechanophysical framework to upscale such properties in multiphase and multiscale materials. These micromechanical modelsare based on the pioneering work of Eshelby , which considers an ellipsoidal inclusion embedded in an infinite isotropic matrix. From the homogenized conductivity viewpoint, the system of randomly oriented anisotropic ellipsoidal inclusions embedded in an isotropic matrix with perfect interfaces between matrix and inclusions KM
v is indistinguishable from the system of spherical inclusions with a volume thermal conductivity Kv (see the Supplemental Material  for the derivations of micromechanics models). Therefore, after proper orientational averaging, the homog-enized thermal conductivity of matrix-inclusion morphol-ogy (known as the Mori-Tanaka scheme)KMT
v reduces to KMTv ¼ fMKMv þ Pnp s¼1fsKsvAsphs fM v þ Pnp s¼1fsA sph s ; ð22Þ where np, fs, and A sph s ¼3KMv=ð2KMv þKsvÞ are, respec-tively, the number of inclusion phases, the volume fraction, and the spherical localization factor of the sth phase. Similarly, the homogenized thermal conductivity for self-consistent morphologyKSC v reduces to KSC v ¼ Pnp s¼1fsKsvB sph s Pnp s¼1fsB sph s ; ð23Þ
where Bsphs ¼3KSCv =ð2KSCv þKsvÞ is the spherical locali-zation factor of thesth phase. It is instructive to note that the mathematical formula for KSC
v has an implicit nature requiring an iterative procedure to obtain the solutions.
As discussed in Sec. I and schematically shown in Fig. 1(b), the CSH paste at the mesoscale is assumed to be comprised of randomly oriented polydisperse CSH
particles with an average size of roughly 5 nm. The characteristic length of these nanoparticles is much smaller than the size of the microscale representative elementary volume and much larger than the mean free path of phonons in the order of Si—O and Ca—O bonds. This means that the conditions of scale separability are fully met between the nano-, meso-, and microscales. Therefore, the microthermoporomechanics formulation introduced above is suitable for homogenization of thermal conductivity of CSH at the mesoscale. Based on the results presented in Fig. 6, the principal thermal-conductivity values of CSH are normally distributed and uncorrelated. Hence, we can treat Eq. (23) in a probabilistic fashion by randomly choosing the principal thermal-conductivity values of the CSH particles from normal distributions. Here, we utilize a Monte-Carlo-uncertainty-propagation scheme to measure both the expectations and standard deviations of the homogenized thermal-conductivity values at microscale. Figure8(a)presents the homogenized thermal conductivity of CSH paste at microscale for two limiting cases of fully saturated and dry mesopores, as a function of the CSH packing density,ζ¼1−φ, where φis the mesoporosity. Since the bulk thermal conductivity values of air and water are lower than that of CSH, the thermal conductivity of CSH paste decreases with increasing porosity. Note that in nanoporous media in contact with the outside air, the composition of confined air will not be that of the outside air. When engineering the CSH heat conduction properties, there are two design parameters: the mesostructure design and the saturation degree of mesopores. Constantinides and Ulmshowed that CSH nanoparticles coalesce at 64% and 76% packing fractions, attributing them to low-density (LD) and high-density (HD) CSHs. Given the two limiting saturation levels and the two packing fractions, the upper and lower bounds of CSH paste’s thermal conductivity can be identified. These bounds are displayed by numbered red and black rectangles in Fig.8(a), where the saturated HD (rectangle 1) and dry LD (rectangle 4) CSHs have, respectively, the highest and lowest homogenized thermal conductivity values.
The cement paste at microscale can be assumed to be a multiphase composite consisting of CSH paste embracing anhydrous clinker phases, portlandite, and fluid inside capillary pores [see Fig. 1(c) and relevant discussion in Sec.I]. The microstructure of cement paste at this scale is akin to that of a matrix-inclusion morphology. Therefore, the Mori-Tanaka scheme would be the method of choice for upscaling the thermal conductivity of individual phases at microscale (level 2) to that of macroscale (level 3). Over the course of cement hydration [see Eqs.(20),(21),(18)], the volume fractions of individual phases (fi) (reactant or product) are known from the reaction degree η and their mass densityρi(see TableI). Therefore, the homog-enized thermal conductivity of cement paste can be implicitly expressed in terms of hydration degree and
the thermal-conductivity values of individual phases (TableII) through Eq.(22). Figure8(b)presents the thermal conductivity as a function of hydration degree for resulting cement pastes produced from the hydration of pure C2S and C3S clinkers at differentw=cratios (w=c¼0.3and 0.5) for saturated meso- and micropores compared with experi-mental measurements of Bentz for cement of varying w=c ratio and curing conditions. Here, we focus on later stages of hydration (0.5<η<1) as other modes of heat transport related to dissolution and precipitation mecha-nisms are rather negligible. We observe that the thermal conductivity of cement paste decreases with increasing hydration degree in agreement with experimental observa-tions of Mounanga et al.as a function of hydration time . This is because thermal-conductivity values of clinker phases are higher than those of hydration products (CSH and CH). Figure8(b)indicates that the macroscopic thermal conductivity of cement paste decreases with increasingw=cratio in full agreement with recent experi-ments of Maruyama and Igarashi . While the volume fraction of portlandite decreases with increasingw=cratio, the volume fraction of unreacted water increases. Considering that the thermal conductivity of bulk water is less than that of portlandite, then it would make sense that the thermal conductivity of cement paste at macroscale decreases with increasing w=cratio.
In this work, thermal properties of cement paste are studied via a multiscale bottom-up approach, starting from the nanoscale by calculating properties of individual constituent phases and connecting them to macroscale
properties using mean-field homogenization theories. At the nanoscale, the phonon density of states of CSHs, CH, β-C2S, and C3S and the components’ atomic con-tributions are studied in detail via the diagonalization of the dynamical matrix and velocity autocorrelation functions. Analogous to glassy materials, we find CSH to exhibit excess of vibrational states characterized by the boson peak at the low-frequency region. The position of the boson peak shifts to higher frequencies with increasing CSH density or, equivalently, by decreasing the Ca∶Si ratio. The constant volume and pressure specific-heat capacities are calculated for individual phases including 11-Å tobermorite. We find that the specific-heat capacity of dry and saturated CSH models increases linearly with the Ca∶Si ratio. The apparent heat capacity of nanoconfined water in the interlayer spacing of CSH is determined to be significantly lower than that of bulk water at room temperature due to strong interaction with the calcium-silicate substrate. We measure the full thermal-conductivity tensor of individual phases using the Green-Kubo relation. The Fourier trans-formation of the heat-flux autocorrelation function reveals long-lasting sharp frequencies associated with optical phonons with zero group velocities that do not contribute to the thermal conduction in these complex systems. In addition, the mean free path of phonons in different phases are estimated to be on the order of Si—O and Ca—O bond lengths. The short mean free path of phonons in the cement-paste-constituent phases meets the condition of scale separability. We demonstrate the variation of the macro-scopic heat capacity of cement paste in terms of the hydration degree using mixture rules. The macroscopic heat-capacity values predicted via our multiscale bottom-up FIG. 8. The mean-field homogenization of thermal conductivity values at the meso- and microscales. (a) The effects of CSH mesostructure (packing density) and saturation degree on the thermal conductivity of CSH paste estimated via probabilistic microthermoporomechanics. (b) The effect of w=c ratio, saturation degree, and the type of clinker phase on macroscale thermal conductivity of hydrating cement paste compared with experimental measurements of Bentzfor hydrating cement pastes.
approach are in good qualitative agreement with experi-ments. We show that the homogenized thermal conduc-tivity of CSH paste at microscale is only affected by the packing density and the saturation level of the CSH mesopores. Our theoretical study indicates that the macro-scopic thermal-conductivity values should decrease with increasing w=c ratio in later stages of hydration degree. Overall, this work provides a bottom-up framework for upscaling thermal properties with potentially broad appli-cations in multiscale and multiphase porous materials.
The Concrete Sustainability Hub at MIT has supported this work with sponsorship provided by the Portland Cement Association (PCA) and the National Ready Mixed Concrete Association (NRMCA) Research and Education Foundation. This work has been partly carried out within the framework of the ICoME2 Labex (ANR-11-LABX-0053) and the A*MIDEX projects (ANR-11-IDEX-0001-02), cofunded by the French program “Investissements d’Avenir,” which is managed by the ANR, the French National Research Agency. With great pleasure, we acknowledge discussions with Dr. Davoud Ebrahimi, Dr. Konrad Krakowiak, Dr. Andrej Kosmirlj, Dr. Andres Saul, Dr. Benoit Coasne, Dr. Jeff Thomas, Dr. Mathieu Bauchy, and Prof. Hamlin Jennings, Prof. Henri Vandamme, and Prof. Sidney Yip.
 F. Ulm and O. Coussy, What is a “massive” concrete structure at early ages? Some dimensional arguments, J. Eng. Mech.127, 512 (2001).
 Mohammad Javad Abdolhosseine Qomi, Arash Noshadravan, Jake Sobstyl, Jameson Toole, J. Ferreira, R. J.-M. Pellenq, F.-J. Ulm, and Marta C. Gonzalez,
“Data Analytics for Energy Efficient Retrofits of Cities” (unpublished).
 G. De Schutter and L. Taerwe, Specific heat and thermal diffusivity of hardening concrete, Mag. Concr. Res. 47, 203 (1995).
 Kook-Han Kim, Sang-Eun Jeon, Jin-Keun Kim, and Sungchul Yang, An experimental study on thermal con-ductivity of concrete,Cem. Concr. Res.33, 363 (2003).  Ramazan Demirboga and Rustem Gul, The effects of
expanded perlite aggregate, silica fume and fly ash on the thermal conductivity of lightweight concrete, Cem. Concr. Res.33, 723 (2003).
 Ramazan Demirboga, Influence of mineral admixtures onˇ thermal conductivity and compressive strength of mortar, Energy Build.35, 189 (2003).
 D. P. Bentz, Transient plane source measurements of the thermal properties of hydrating cement pastes, Mater. Construc. Mater. Structures40, 1073 (2007).
 Seyoon Yoon, Donald E. Macphee, and Mohammed S. Imbabi, Estimation of the thermal properties of hardened
cement paste on the basis of guarded heat flow meter measurements,Thermochim. Acta 588, 1 (2014).  D. Mikulic, B. Milovanovic, and I. Gabrijel, in
Nondestru-ctive Testing of Materials and Structures, RILEM Books-eries Vol. 6, edited by Oguz Gunes and Yılmaz Akkaya (Springer Netherlands, Dordrecht, 2013) pp. 465–471.  Ippei Maruyama and Go Igarashi, Cement reaction and
resultant physical properties of cement paste, J. Adv. Concr. Technol. 12, 200 (2014).
 Yunsheng Xu and D. D. L. Chung, Effect of sand addition on the specific heat and thermal conductivity of cement, Cem. Concr. Res.30, 59 (2000).
 A. Abdelalim, S. Abdallah, K. Easawi, S. Negm, and H. Talaat, Thermal properties of hydrated cement pastes studied by the photoacoustic technique, J. Phys. Conf. Ser.214, 012136 (2010).
 E. Masoero, E. Del Gado, R. J.-M. Pellenq, F.-J. Ulm, and S. Yip, Nanostructure and Nanomechanics of Cement: Polydisperse Colloidal Packing, Phys. Rev. Lett. 109, 155503 (2012).
 Andrew J. Allen, Jeffrey J. Thomas, and Hamlin M. Jennings, Composition and density of nanoscale calcium-silicate-hydrate in cement,Nat. Mater.6, 311 (2007).  W.-S. Chiang, G. Ferraro, E. Fratini, F. Ridi, Y.-Q. Yeh,
U-S. Jeng, S.-H. Chen, and P. Baglioni, Multiscale structure of calcium- and magnesium-silicate-hydrate gels, J. Mater. Chem. A2, 12991 (2014).
 Georgios Constantinides and Franz-Josef Ulm, The nano-granular nature of C-S-H, J. Mech. Phys. Solids 55, 64 (2007).
 Luc Dormieux, Djimedo Kondo, and Franz-Jozef Ulm, Microporomechanics, 1st ed. (Wiley, Hoboken, NJ, 2006).
 M. J. Abdolhosseini Qomi, K. J. Krakowiak, M. Bauchy, K. L. Stewart, R. Shahsavari, D. Jagannathan, D. B. Brommer, A. Baronnet, M. J. Buehler, S. Yip, F.-J. Ulm, K. J. Van Vliet, and R. J.-M. Pellenq, Combinatorial molecular optimization of cement hydrates,Nat. Commun.
5, 4960 (2014).
 M. Bauchy, M. J. Abdolhosseini Qomi, F.-J. Ulm, and R. J.-M. Pellenq, Order and disorder in calcium-silicate-hydrate,J. Chem. Phys.140, 214503 (2014).
 Mathieu Bauchy, Mohammad Javad Abdolhosseini Qomi, Christophe Bichara, Franz-Joseph Ulm, and Roland J.-M. Pellenq, Nanoscale structure of cement: Viewpoint of rigidity theory,J. Phys. Chem. C 118, 12485 (2014).  M. Bauchy, M. J. Abdolhosseini Qomi, C. Bichara, F.-J.
Ulm, and R. J.-M. Pellenq,arXiv:1410.2916.
 M. Bauchy, H. Laubie, M. J. Abdolhosseini Qomi, C. G. Hoover, F.-J. Ulm, and R. J.-M. Pellenq, Fracture tough-ness of calcium-silicate-hydrate from molecular dynamics simulations,J. Non-Cryst. Solids419, 58 (2015).  Mathieu Bauchy, Mohammad Javad Abdolhosseine Qomi,
Christophe Bichara, F. J. Ulm, and Roland J.-M. Pellenq, Rigidity Transition in Materials: Hardness Is Driven by Weak Atomic Constraints, Phys. Rev. Lett. 114, 125502 (2015).
 Mohammad Javad Abdolhosseini Qomi, Mathieu Bauchy, Franz-Josef Ulm, and Roland J.-M. Pellenq, Anomalous composition-dependent dynamics of nanoconfined water